Electroplating - wikipedia Electroplating Copper electroplating machine for layering PCBs Electroplating is a process that uses electric current to reduce dissolved metal cations so that they form a thin coherent metal coating on an electrode. The term is also used for electrical oxidation of anions on to a solid substrate, as in the formation of silver chloride on silver wire to make silver / silver - chloride electrodes. Electroplating is primarily used to change the surface properties of an object ( such as abrasion and wear resistance, corrosion protection, lubricity, aesthetic qualities ), but may also be used to build up thickness on undersized parts or to form objects by electroforming. The process used in electroplating is called electrodeposition. It is analogous to a concentration cell acting in reverse. The part to be plated is the cathode of the circuit. In one technique, the anode is made of the metal to be plated on the part. Both components are immersed in a solution called an electrolyte containing one or more dissolved metal salts as well as other ions that permit the flow of electricity. A power supply supplies a direct current to the anode, oxidizing the metal atoms that it comprises and allowing them to dissolve in the solution. At the cathode, the dissolved metal ions in the electrolyte solution are reduced at the interface between the solution and the cathode, such that they `` plate out '' onto the cathode. The rate at which the anode is dissolved is equal to the rate at which the cathode is plated, vis - à - vis the current through the circuit. In this manner, the ions in the electrolyte bath are continuously replenished by the anode. Other electroplating processes may use a nonconsumable anode such as lead or carbon. In these techniques, ions of the metal to be plated must be periodically replenished in the bath as they are drawn out of the solution. The most common form of electroplating is used for creating coins, such as US pennies, which are made of zinc covered in a layer of copper. Contents 1 Process 1.1 Strike 1.2 Electrochemical deposition 1.3 Pulse electroplating or pulse electrodeposition ( PED ) 1.4 Brush electroplating 1.5 Electroless deposition 1.6 Cleanliness 2 Effects 3 History 4 Uses 5 Hull cell 6 Haring -- Blum cell 7 See also 8 References 8.1 Bibliography 9 External links Process Electroplating of a metal ( Me ) with copper in a copper sulphate bath See also : Electrotyping and Electroforming The cations associate with the anions in the solution. This cations are reduced at the cathode to deposit in the metallic, zero valence state. For example, for copper plating, in an acid solution, copper is oxidized at the anode to Cu by losing two electrons. The Cu associates with the anion SO in the solution to form copper ( II ) sulphate. At the cathode, the Cu is reduced to metallic copper by gaining two electrons. The result is the effective transfer of copper from the anode source to a plate covering the cathode. The plating is most commonly a single metallic element, not an alloy. However, some alloys can be electrodeposited, notably brass and solder. Many plating baths include cyanides of other metals ( such as potassium cyanide ) in addition to cyanides of the metal to be deposited. These free cyanides facilitate anode corrosion, help to maintain a constant metal ion level and contribute to conductivity. Additionally, non-metal chemicals such as carbonates and phosphates may be added to increase conductivity. When plating is not desired on certain areas of the substrate, stop - offs are applied to prevent the bath from coming in contact with the substrate. Typical stop - offs include tape, foil, lacquers, and waxes. The ability of a plating to cover uniformly is called throwing power ; the better the throwing power the more uniform the coating. Strike Initially, a special plating deposit called a strike or flash may be used to form a very thin ( typically less than 0.1 μm thick ) plating with high quality and good adherence to the substrate. This serves as a foundation for subsequent plating processes. A strike uses a high current density and a bath with a low ion concentration. The process is slow, so more efficient plating processes are used once the desired strike thickness is obtained. The striking method is also used in combination with the plating of different metals. If it is desirable to plate one type of deposit onto a metal to improve corrosion resistance but this metal has inherently poor adhesion to the substrate, a strike can be first deposited that is compatible with both. One example of this situation is the poor adhesion of electrolytic nickel on zinc alloys, in which case a copper strike is used, which has good adherence to both. Electrochemical deposition Electrochemical deposition is generally used for the growth of metals and conducting metal oxides because of the following advantages : the thickness and morphology of the nanostructure can be precisely controlled by adjusting the electrochemical parameters ; relatively uniform and compact deposits can be synthesized in template - based structures ; higher deposition rates are obtained ; and the equipment is inexpensive due to the non-requirements of either a high vacuum or a high reaction temperature. Pulse electroplating or pulse electrodeposition ( ped ) A simple modification in electroplating is pulse electroplating. This process involves the swift alternating of the potential or current between two different values resulting in a series of pulses of equal amplitude, duration and polarity, separated by zero current. By changing the pulse amplitude and width, it is possible to change the deposited film 's composition and thickness. The experimental parameters of pulse electroplating usually consist of peak current / potential, duty cycle, frequency and effective current / potential. Peak current / potential is the maximum setting of electroplating current or potential. Duty cycle is the effective portion of time in certain electroplating period with the current or potential applied. The effective current / potential is calculated by multiplying the duty cycle and peak value of current or potential. Pulse electroplating could help to improve the quality of electroplated film and release the internal stress built up during fast deposition. Combination of the short duty cycle and high frequency could decrease the surface cracks. However, in order to maintain the constant effective current or potential, a high performance power supply may be required to provide high peak current / potential and fast switch. Another common problem of pulse electroplating is that the anode material could get plated and contaminated during the reverse electroplating, especially for the high cost, inert electrode like platinum. Other factors that could affect the pulse electroplating include temperature, anode - to - cathode gap and stirring. Sometimes the pulse electroplating can be performed in heated electroplating bath to increase the depositing rate since the rate of almost all the chemical reaction increases exponentially with temperature per Arrhenius law. The anode - to - cathode gap is related to the current distribution between anode and cathode. Small gap to sample area ratio may cause uneven distribution of current and affect the surface topology of plated sample. Stirring may increase the transfer / diffusion rate of metal ions from bulk solution to the electrode surface. Stirring setting varies for different metal electroplating processes. Brush electroplating A closely related process is brush electroplating, in which localized areas or entire items are plated using a brush saturated with plating solution. The brush, typically a stainless steel body wrapped with an absorbent cloth material that both holds the plating solution and prevents direct contact with the item being plated, is connected to the anode of a low voltage direct current power source, and the item to be plated connected to the cathode. The operator dips the brush in plating solution then applies it to the item, moving the brush continually to get an even distribution of the plating material. Brush electroplating has several advantages over tank plating, including portability, ability to plate items that for some reason can not be tank plated ( one application was the plating of portions of very large decorative support columns in a building restoration ), low or no masking requirements, and comparatively low plating solution volume requirements. Disadvantages compared to tank plating can include greater operator involvement ( tank plating can frequently be done with minimal attention ), and inability to achieve as great a plate thickness. Electroless deposition Usually an electrolytic cell ( consisting of two electrodes, electrolyte, and external source of current ) is used for electrodeposition. In contrast, electroless deposition uses only one electrode and no external source of electric current. However, the solution for electroless deposition needs to contain a reducing agent so that the electrode reaction has the form : M z + + Red solution → catalytic surface M solid + Oxy solution ( displaystyle ( ce ( ( M ^ ( mathit ( z ) ) + ) + Red_ ( solution ) - > ( ( ce ( catalytic ~ surface ) ) ) ( M_ ( solid ) ) + Oxy_ ( solution ) ) ) ) In principle any hydrogen - based reducing agent can be used although the redox potential of the reducing half - cell must be high enough to overcome the energy barriers inherent in liquid chemistry. Electroless nickel plating uses hypophosphite as the reducer while plating of other metals like silver, gold and copper typically use low - molecular - weight aldehydes. A major benefit of this approach over electroplating is that the power sources and plating baths are not needed, reducing the cost of production. This technique can also plate diverse shapes and types of surface. The downside is that plating is usually slower and can not create thick plates of metal. As a consequence of these characteristics, electroless deposition is quite common in the decorative arts. Cleanliness Cleanliness is essential to successful electroplating, since molecular layers of oil can prevent adhesion of the coating. ASTM B322 is a standard guide for cleaning metals prior to electroplating. Cleaning includes solvent cleaning, hot alkaline detergent cleaning, electrocleaning, and acid treatment etc. The most common industrial test for cleanliness is the waterbreak test, in which the surface is thoroughly rinsed and held vertical. Hydrophobic contaminants such as oils cause the water to bead and break up, allowing the water to drain rapidly. Perfectly clean metal surfaces are hydrophilic and will retain an unbroken sheet of water that does not bead up or drain off. ASTM F22 describes a version of this test. This test does not detect hydrophilic contaminants, but electroplating can displace these easily since the solutions are water - based. Surfactants such as soap reduce the sensitivity of the test and must be thoroughly rinsed off. Effects Electroplating changes the chemical, physical, and mechanical properties of the workpiece. An example of a chemical change is when nickel plating improves corrosion resistance. An example of a physical change is a change in the outward appearance. An example of a mechanical change is a change in tensile strength or surface hardness which is a required attribute in tooling industry. Electroplating of acid gold on underlying copper - or nickel - plated circuits reduces contact resistance as well as surface hardness. Copper - plated areas of mild steel act as a mask if case hardening of such areas are not desired. Tin - plated steel is chromium - plated to prevent dulling of the surface due to oxidation of tin. Electroplating, or electroless plating may be used as a way to render a metal part radioactive, by using an aqueous solution prepared from nickel -- phosphorus concentrates which contain radioactive hypophosphite P ions. Such a part might be used for the purposes of brachytherapy. History Luigi Valentino Brugnatelli ( it ) Boris Jacobi developed electroplating, electrotyping and galvanoplastic sculpture in Russia Nickel plating See also : Johann Wilhelm Ritter Modern electrochemistry was invented by Italian chemist Luigi Valentino Brugnatelli ( it ) in 1805. Brugnatelli used his colleague Alessandro Volta 's invention of five years earlier, the voltaic pile, to facilitate the first electrodeposition. Brugnatelli 's inventions were suppressed by the French Academy of Sciences and did not become used in general industry for the following thirty years. By 1839, scientists in Britain and Russia had independently devised metal - deposition processes similar to Brugnatelli 's for the copper electroplating of printing press plates. Boris Jacobi in Russia not only rediscovered galvanoplastics, but developed electrotyping and galvanoplastic sculpture. Galvanoplastics quickly came into fashion in Russia, with such people as inventor Peter Bagration, scientist Heinrich Lenz and science fiction author Vladimir Odoyevsky all contributing to further development of the technology. Among the most notorious cases of electroplating usage in mid-19th century Russia were gigantic galvanoplastic sculptures of St. Isaac 's Cathedral in Saint Petersburg and gold - electroplated dome of the Cathedral of Christ the Saviour in Moscow, the tallest Orthodox church in the world. Galvanoplastic sculpture on St. Isaac 's Cathedral in Saint Petersburg. The Woolrich Electrical Generator in Thinktank, Birmingham Soon after, John Wright of Birmingham, England discovered that potassium cyanide was a suitable electrolyte for gold and silver electroplating. Wright 's associates, George Elkington and Henry Elkington were awarded the first patents for electroplating in 1840. These two then founded the electroplating industry in Birmingham from where it spread around the world. The Woolrich Electrical Generator of 1844, now in Thinktank, Birmingham Science Museum, is the earliest electrical generator used in industry. It was used by Elkingtons. The Norddeutsche Affinerie in Hamburg was the first modern electroplating plant starting its production in 1876. As the science of electrochemistry grew, its relationship to electroplating became understood and other types of non-decorative metal electroplating were developed. Commercial electroplating of nickel, brass, tin, and zinc were developed by the 1850s. Electroplating baths and equipment based on the patents of the Elkingtons were scaled up to accommodate the plating of numerous large scale objects and for specific manufacturing and engineering applications. The plating industry received a big boost with the advent of the development of electric generators in the late 19th century. With the higher currents available, metal machine components, hardware, and automotive parts requiring corrosion protection and enhanced wear properties, along with better appearance, could be processed in bulk. The two World Wars and the growing aviation industry gave impetus to further developments and refinements including such processes as hard chromium plating, bronze alloy plating, sulfamate nickel plating, along with numerous other plating processes. Plating equipment evolved from manually operated tar - lined wooden tanks to automated equipment, capable of processing thousands of kilograms per hour of parts. One of the American physicist Richard Feynman 's first projects was to develop technology for electroplating metal onto plastic. Feynman developed the original idea of his friend into a successful invention, allowing his employer ( and friend ) to keep commercial promises he had made but could not have fulfilled otherwise. Uses Electroplating is widely used in various industries for coating metal objects with a thin layer of a different metal. The layer of metal deposited has some desired property, which the metal of the object lacks. For example, chromium plating is done on many objects such as car parts, bath taps, kitchen gas burners, wheel rims and many others for the fact that chromium is very corrosion - resistant, and thus prolongs the life of the parts. It is also used in making expensive jewelry. Hull cell A zinc solution tested in a Hull cell The Hull cell is a type of test cell used to qualitatively check the condition of an electroplating bath. It allows for optimization for current density range, optimization of additive concentration, recognition of impurity effects and indication of macro-throwing power capability. The Hull cell replicates the plating bath on a lab scale. It is filled with a sample of the plating solution, an appropriate anode which is connected to a rectifier. The `` work '' is replaced with a Hull cell test panel that will be plated to show the `` health '' of the bath. The Hull cell is a trapezoidal container that holds 267 mL of solution. This shape allows one to place the test panel on an angle to the anode. As a result, the deposit is plated at different current densities which can be measured with a hull cell ruler. The solution volume allows for a quantitative optimization of additive concentration : 1 gram addition to 267 mL is equivalent to 0.5 oz / gal in the plating tank. Haring -- Blum cell Haring -- Blum cell The Haring -- Blum cell is used to determine the macro throwing power of a plating bath. The cell consists of two parallel cathodes with a fixed anode in the middle. The cathodes are at distances from the anode in the ratio of 1 : 5. The macro throwing power is calculating from the thickness of plating at the two cathodes when a direct current is passed for a specific period of time. The cell is fabricated out of perspex or glass. See also Nanolamination Electrochemical engineering References Jump up ^ Dufour, 2006 & IX - 1. ^ Jump up to : Dufour, 2006 & IX - 2 Jump up ^ `` US Mint Virtual Tour ''. US Mint. Archived from the original on 2012 - 11 - 02. Jump up ^ Dufour 2006, p. IX - 3 Jump up ^ `` Pollution Prevention Technology Profile Trivalent Chromium Replacements for Hexavalent Chromium Plating '' ( PDF ). Northeast Waste Management Officials ' Association. 2003 - 10 - 18. Archived from the original ( PDF ) on 2010 - 08 - 06. Jump up ^ US 4882014, Coyle, R.T. & J.A. Switzer, `` Electrochemical synthesis of ceramic films and powders '' Jump up ^ Gal - Or, L. ; Silberman, I. ; Chaim, R. ( 1991 ). `` Electrolytic ZrO Coatings : I. Electrochemical Aspects ''. Journal of the Electrochemical Society. 138 ( 7 ) : 1939. doi : 10.1149 / 1.2085904. Jump up ^ Ju, Hyungkuk ; Lee, Jae - Kwang ; Lee, Jongmin ; Lee, Jaeyoung ( 2012 ). `` Fast and selective Cu O nanorod growth into anodic alumina templates via electrodeposition ''. Current Applied Physics. 12 : 60. doi : 10.1016 / j. cap. 2011.04. 042. Jump up ^ Chandrasekar, M.S. ; Pushpavanam, Malathy ( 2008 ). `` Pulse and pulse reverse plating -- Conceptual, advantages and applications ''. Electrochimica Acta. 53 ( 8 ) : 3313 -- 3322. doi : 10.1016 / j. electacta. 2007.11. 054. Jump up ^ Todd, Robert H. ; Allen, Dell K. ; Alting, Leo ( 1994 ). `` Surface Coating ''. Manufacturing Processes Reference Guide. Industrial Press. pp. 454 -- 458. ISBN 0 - 8311 - 3049 - 0. Archived from the original on 2013 - 10 - 09. Jump up ^ US 6475644, Hampikian, Janet & Neal Scott, `` Radioactive coating solutions methods, and substrates '' Jump up ^ `` The history of galvanotechnology in Russia ''. Archived from the original on March 5, 2012. ( in Russian ) Jump up ^ Birmingham Museums trust catalogue, accession number : 1889S00044 Jump up ^ Thomas, John Meurig ( 1991 ). Michael Faraday and the Royal Institution : The Genius of Man and Place. Bristol : Hilger. p. 51. ISBN 0750301457. Jump up ^ Beauchamp, K.G. ( 1997 ). Exhibiting Electricity. IET. p. 90. ISBN 9780852968956. Jump up ^ Hunt, L.B. ( March 1973 ). `` The early history of gold plating ''. Gold Bulletin. 6 ( 1 ) : 16 -- 27. doi : 10.1007 / BF03215178. Jump up ^ Stelter, M. ; Bombach, H. ( 2004 ). `` Process Optimization in Copper Electrorefining ''. Advanced Engineering Materials. 6 ( 7 ) : 558. doi : 10.1002 / adem. 200400403. Jump up ^ Feynman, Richard ( 1985 ). `` Chapter 6 : The Chief Research Chemist of the Metaplast Corporation ''. Surely You 're Joking, Mr. Feynman !. Jump up ^ Metal Finishing : Guidebook and Directory. Issue 98. 95. 1998. p. 588. Jump up ^ Kushner, Arthur S. ( December 1, 2006 ). `` Hull Cell 101 ''. Products Finishing. Archived from the original on March 13, 2010. Jump up ^ Bard, Allan ; Inzelt, György ; Scholz, Fritz ( 2012 ). `` Haring -- Blum Cell ''. Electrochemical Dictionary. Springer. p. 444. doi : 10.1007 / 978 - 3 - 642 - 29551 - 5_8. ISBN 978 - 3 - 642 - 29551 - 5. Jump up ^ Wendt, Hartmut ; Gerhard, Kreyse ( 1999 ). Electrochemical Engineering : Science and Technology in Chemical and Other Industries. Springer. p. 122. ISBN 3540643869. Bibliography Dufour, Jim ( 2006 ). An Introduction to Metallurgy ( 5th ed. ). Cameron. External links Real electroplating on PTH - treated electroless copper plating on YouTube Metalworking Casting Processes Centrifugal Continuous Die Evaporative - pattern Full mold Lost foam Investment ( Lost wax ) Permanent mold Plaster mold Sand Semi-solid metal Shaw process Shell molding Spin Components Chill Cope and drag Core Flask Molding sand Pattern Riser Sprue Terminology Casting defects Draft Dross Ingot Semi-finished casting products Slag Forming, fabrication, and finishing General Fabrication Piece work Sheet metal Forming processes Coining Drawing Electrohydraulic forming Electromagnetic forming Explosive forming Forging Hydroforming Progressive stamping Punching Rolling Sinking Spinning Swaging Tube bending Joining processes Brazing Crimping Riveting Soldering Welding Finishing processes Anodizing Galvanizing Heat treating Mass finishing Patination Peening Plating Polishing Machining and computing Computer - aided engineering 2.5 D CAD CAM G - code Numerical control ( NC and CNC ) Stewart platform Drilling and threading Die head Drill Drill bit Drill bit shank Drill bit sizes Drilling List of drill and tap sizes Tap and die Tap wrench Threading Grinding and lapping Abrasive Angle grinder Bench grinder Coated abrasives Cylindrical grinder Diamond plate Flick grinder Grinding Grinding dresser Grinding machine Grinding wheel Jig grinder Lapping Sanding Sharpening stone Spark testing Surface grinder Tool and cutter grinder Machining Boring Broaching Electrical discharge machining Electrochemical machining Electron beam machining Endmill Engraving Facing Hobbing Jig borer Machine tool Machining Metal lathe Milling cutter Milling machine Pantograph Photochemical machining Planer Reamer Rotary transfer machine Shaper Turning Ultrasonic machining Machine tooling Angle plate Chuck Collet Fixture Indexing head Jig Lathe center Machine taper Magnetic base Mandrel Rotary table Wiggler Terminology Cutting fluid Machining vibrations Speeds and feeds Swarf Tolerance Tool and die making Tramp oil Smithing Smiths Blacksmith Bladesmith Coppersmith Goldsmith Gunsmith Locksmith Pewtersmith Silversmith Tinsmith Processes Forging Pattern welding Planishing Raising Sinking Swaging Tools Anvil Forge Fuller Hammer Hardy tools Pritchel Steam hammer Swage block Trip hammer Tools Cutting machines Bandsaw Cold saw Laser Miter saw Plasma Water jet cutter Cutting tools Broach Burr Chisel Counterbore Countersink End mill File Hand scraper Milling cutter Nibbler Reamer Shears Tipped tool Tool bit Forming tools Brake Die English wheel Hydraulic press Machine press Punch press Screw press Stamping press Hand tools Clamp Combination square Drift pin Hacksaw Hammer Hand scraper Machinist square Needlegun scaler Piercing saw Pliers Punch Scriber Tap and die Tongs Vise Workbench Wrench Machine tooling Angle plate Chuck Collet Fixture Indexing head Jig Lathe center Machine taper Magnetic base Mandrel Rotary table Wiggler Measuring instruments Bore gauge Caliper Center gauge Dial indicator Engineer 's blue Engineer 's spirit level Feeler gauge Gauge Gauge block Go / no go gauge Height gauge Machinist square Marking blue Marking gauge Marking out Micrometer Optical comparator Radius gauge Ruler Sine bar Straightedge Surface plate Tape measure Thread pitch gauge Vernier scale Smithing tools Anvil Forge Fuller Hardy tools Pritchel Steam hammer Swage block Trip hammer Welding Arc welding Atomic hydrogen ( Athydo / AHW ) Electrogas ( EGW ) Flash Flux - cored ( FCAW ) Gas metal ( Microwire / MIG / GMAW ) Gas tungsten ( Heliarc / TIG / GTAW ) Plasma ( PAW ) Shielded metal ( Stick / MMA / SMAW ) Submerged ( SAW ) Other processes Electric resistance ( ERW ) Electron beam ( EBW ) Electroslag ( ESW ) Exothermic Forge Friction Friction stir ( FSW ) Friction stud Laser beam ( LBW ) Laser - hybrid Magnetic pulse Oxyacetylene ( OAW ) Spot ( RSW ) Ultrasonic Upset Equipment Electrode Filler metal Helmet Power supply Robot Shielding gas Related terms Heat - affected zone Photokeratitis Residual stress Weldability Casting Fabrication Forming Jewellery Machining Metallurgy Smithing Tools and terminology Welding Retrieved from `` https://en.wikipedia.org/w/index.php?title=Electroplating&oldid=840988639 '' Categories : Metal plating Hidden categories : Articles with Russian - language external links Wikipedia articles needing clarification from April 2015 Interlanguage link template link number Pages with missing ISBNs Talk Contents About Wikipedia Tools Afrikaans Azərbaycanca Català Dansk Deutsch Eesti Español Esperanto Euskara Français हिन्दी Hrvatski Italiano Кыргызча Magyar മലയാളം Bahasa Melayu Монгол Nederlands नेपाली 日本 語 Norsk Norsk nynorsk ਪੰਜਾਬੀ Polski Русский Simple English Srpskohrvatski / српскохрватски Svenska Тыва дыл Українська 粵語 中文 25 more Edit links This page was last edited on 13 May 2018, at 10 : 13. Text is available under the Creative Commons Attribution - ShareAlike License ; additional terms may apply. By using this site, you agree to the Terms of Use and Privacy Policy. Wikipedia ® is a registered trademark of the Wikimedia Foundation, Inc., a non-profit organization. About Wikipedia

Question: give two examples of the application of electroplating
Answer: car parts